5. CIGS by Low-Temperature PED for TFSCs
5.3. PED-CIGS solar cells architecture
In this thesis, the structure of devices based on CIGS grown by LTPED were changed in function of the study carried out. The classic CIGS-based solar cell structure is shown in Figure 5.14.
Figure 5.14 – Classic structure of a solar cell based on CIGS.
Here, the materials stacked up in typical architecture are described, along with their deposition processes. This classic structure is used to fabricate the present LTPED record solar cell and for the combinatorial PED study.
Architecture variations are performed to realize bifacial solar cells and Cd-free devices. The characteristics and deposition methods of TCOs as back contact and Zn(O,S) buffer layer are described in chapter 6. and chapter 7. , respectively.
5.3.1. Substrate and back contact
The substrates were commercial 2mm-thick 2.5cm×2.5cm (6.25 cm2) soda-lime glass, covered with Si3N4 and Mo, supplied by Singulus Technologies. Si3N4 had a thickness of 100 nm and acted as blocking layer to avoid sodium diffusion from the glass into the CIGS, thereby the sodium content was controlled by the NaF precursor layer only. Mo layer is 700nm-thick deposited by sputtering and was the back contact of the solar cells, with a sheet resistance of 35 μΩ/sq.
For the TCO study of chapter 6. , Al:ZnO and ITO by RF-Magnetron sputtering on SLG and commercial FTO on SLG were used as back contact.
In the study about the alternative buffer layer, for co-evaporated CIGS only, Mo back contact was DC-sputtered onto SLG.
5.3.2. Sodium precursor
The low temperature of PED process was found to start an uncontrolled and non-optimized Na migration from the SLG substrate, through the Mo back contact, into CIGS. Therefore, to control the supply of sodium to the absorber, NaF was deposited by PED directly onto the back contact, immediately before the CIGS deposition. The NaF thickness determined the amount of sodium incorporated in the CIGS. A Si3N4 diffusion barrier was introduced between SLG and Mo to avoid any glass contribution.
NaF was deposited on Mo using PED voltage of 14 kV with a repetition rate of 10Hz, at an Ar pressure of 5∙10-3 mbar. The substrate temperature was kept at 80 °C and the distance target-substrate is the same as CIGS: 8 cm. Target cleaning was performed shooting 2k pulses before the deposition, the substrate still parked in the load lock. From time to time, a thickness calibration was carried out to determine any variation in the NaF deposition rate, mainly due to the target getting thinner: 5k pulses were shot on glass and the film thickness was measured by profilometer. The NaF deposition rate was about 0.02 nm/pulse. A calibrated thickness of 8-10 nm was then deposited onto Mo in a few hundreds of pulses.
The low temperature of Mo substrate during the CIGS deposition does not allow the formation of MoSe2
compound between CIGS and Mo, as SIMS analyses of Figure 5.12 confirmed: no peak of Se signal (pinkish curve) was observed close to the Mo layer. The interface CIGS/Mo is known to be a Schottky barrier to holes, whose large height affects both FF and Voc of the solar cells. Then, MoSe2 layer is very important because it attenuates the band distortion at the interface lowering the barrier height, hence forming a quasi-ohmic contact which minimizes the losses. (62) (63) (64) In PED deposition of CIGS, a new route to obtain an ohmic contact must be applied. The deposition of NaF prior to the CIGS growth was found to be a good alternative to the MoSe2 layer. To investigate the electrical behaviour of CIGS/Mo back-contact, Au/CIGS/Mo and Au/CIGS/NaF/Mo structures on glass substrates were prepared. The Au/CIGS contacts were used to ensure a sufficient ohmic characteristics of the top contact (65) and to allow the detection of the resistivity changes at the back contact. The measured JV curves of both structures are reported in Figure 5.15 and clearly show the transition from rectifying to ohmic behaviour when introducing the NaF layer. These results explained why series resistances as low as 0.2 Ω/cm2can be achieved in solar cells grown at substrate temperatures as low as 250 °C, in the presence of a NaF buffer layer on top of the Mo back-contact. Coupled to the poor sodium diffusion due to the low temperature, the NaF layer provides a high sodium content into the first CIGS region, increasing the free-hole density therein. The proposed mechanism supposes that the high doping of CIGS can thin the barrier enough to be tunnelled by carriers. This could be the reason why good device quality (as shown in the next sections of this chapter) could be obtained with the LTPED growth of CIGS on Mo, even if MoSe2 is not formed.
Figure 5.15 – Current density vs voltage behaviour of a) Au/CIGS/Mo structure and b) Au/CIGS/NaF/Mo one. The introduction of the sodium precursor layer(NaF) turned the CIGS/Mo rectifing junction into ohmic contact, for both dark
(red curve) and illuminated line (blue curve). (55)
If the low substrate temperature is not a problem for the formation of the back ohmic contact, sodium diffusion into the CIGS film at 250 °C is much less effective compared to CIGS cells grown and annealed at temperatures as high as 600 °C. Increasing the thickness of the NaF buffer layer to enhance Na diffusion is not an option as CIGS adhesion on Mo is compromised by a NaF thickness exceeding a critical value of about 30 nm. In the case of the basic CIGS solar cells, the CIGS film thickness was limited to 1.6 μm even to ensure an optimum sodium diffusion through the whole absorber, for 8-10 nm of NaF. Alternative solutions were explored at IMEM-CNR to incorporate Na or to tune its diffusion profile and extend the diffusion range, without exceeding the critical Na concentration in CIGS:
providing NaF after the CIGS deposition has resulted in a poor contact between Mo and CIGS and might even cause a high doping of CIGS in the space-charge region, which lowers the SCR extension.
NaF inclusion into the CIGS target was a good solution to ablate both the materials at the same time and to build a flat sodium profile inside the CIGS, but had been found to result in bad target homogeneity: NaF phases has separated from CIGS and the evaporating ratio of the two materials was completely random.
Introducing sodium into the middle of CIGS had caused both bad contacts towards Mo and huge problems to mechanical stability of CIGS: an incomplete NaF diffusion had probably resulted in great quantity of sodium at the grain boundary, that later caused the peel off. The thickness limit for NaF layer included into CIGS film must be very thin not to cause grains disaggregation.
A more elegant approach to overcome the poor Na diffusion can be the deposition of a NaF/CIGS multilayer structure by PED, maintaining low temperatures and avoiding long-time annealing process. Its aim is to create a sodium profile providing NaF where it is necessary and taking advantage of the low diffusion to have different content inside CIGS in function of the depth. Preliminary study confirmed that alternating nano-layer of NaF at the CIGS deposition provides an easy way to carefully control the Na content and gradient along the CIGS-growth
direction at temperature as low as 250 °C. Of course, the NaF layers thickness, the distance between them, their number and their position inside CIGS are the parameters to be adjusted to create a Na gradient. This Na gradient could be useful to select the doping of CIGS as a function of the depth from the surface and the width of the space charge region. We believe it is a fundamental step for the optimization of high-quality and large-area thin-film solar cells based on CIGS by PED. This strategy is currently being developed at IMEM-CNR of Parma. (66) 5.3.3. CIGS absorber
The CIGS absorber is grown by the single-stage LTPED process with the set-up described in section 5.1 and the deposition parameters described in section 5.2.
5.3.4. Buffer layer
CdS by chemical bath deposition was used as buffer layer for the solar cell of this chapter and for the study about back contacts made by TCOs. Reference solar cells of Zn(O,S) series were buffered with CdS as well.
CdS grown by CBD has great inclusion of oxygen and hydroxide groups (up to 10% of overall atoms), so the buffer material actually is Cd(S,O,OH). Other impurities like C and N are present in the lattice due to reaction by-products. Both the amount of this impurities and the morphology of CdS depends on the deposition condition: temperature, precursor compounds and their ratio, CIGS surface, and so on.
Post deposition treatment of CIGS with KF nucleates a more uniform film of CdS, thus increasing the Voc and allowing to thin the buffer for a slight enhancement of Jsc. In the present thesis, no KF treatment was applied.
CdS was grown by an in-house CBD process. Stock aqueous solution of 0.1 M cadmium chloride (CdCl2), 0.1 M thiourea (CS(NH2)2) and 16.8 M ammonia (NH3) were stored in tightly closed bottom.
The freshly-grown CIGS sample was introduced into a 100-ml flat-bottom borosilicate-glass beaker containing a room-temperature solution of bi-distilled water (43 ml) and ammonia (15.4 ml) having pH=12, for 5 minutes. Later, the two chemical precursors for CdS deposition were added, still at RT:
first CdCl2 (1.4 ml) followed by thiourea (20 ml) after 2 minutes, with a concentration ratio of about 1:14. Then, the beaker containing sample and solution was introduced in the hot bath at 80 °C to start the CBD process. The beaker was magnetically stirred and after 10 min, the sample was extracted from the solution and the procedure was repeated with a fresh solution. At the end of the second stage, a 90-100nm-thick film of CdS was grown.
The reaction steps are illustrated in Figure 5.16. As soon as the CIGS sample was exposed to air, it was introduced into the ammonia solution with pH=12 for 5 min at room temperature. NH3 is believed to
“clean” the CIGS surface from CO2 deposition and from oxidation occurred during the unavoidable air exposure. Later CdCl2 was introduced in the solution to start the formation of Cd-ammine ion complexes
onto the CIGS surface, which are essential for the CdS nucleation. After 1 min, the solution was putted into the hot bath at 80 °C and thiourea was added. S2- ions are created by the interaction of thiourea with OH- of the solution and when the temperature is risen enough, CdS is formed at a Cd2+:S2- ratio of 1:2.
The nucleation started with islands and their growth brings to the film formation. After about 10 min, the CdS layer was not yet fully covering but big clusters were formed inside the solution and floated on the surface. Their dimension was not comparable to CdS buffer thickness, thereby the sample was extracted from the solution to avoid their inclusion in the film and very-bad buffer morphology. A second deposition with the same parameters was then carried out to obtain a fully covering layer with a thickness of about 90nm. The sample was cleaned with de-ionized water and dried by means of Ar flow.
Figure 5.16 – Growth mechanism of chemical bath deposited CdS (orange) over CIGS (dark grey substrate).
Thickness of 90nm-100nm were found to be the optimal compromise between light absorption and shunt resistance. Lower thickness caused more shunted solar cells, so FF loss. Thicker film indeed enhanced the light absorption of the buffer, hence decreasing the Jsc.
The shunt-preventing layer of the solar cells was made by ~100 nm of i-ZnO, while roughly-800nm-thick film of Al-doped ZnO was the front transparent contact of the devices. They were deposited by means of RF-Magnetron sputtering, using cathode fabricated by Angstrom Science. Commercial targets by Testbourne Ltd. were used, produced by Hot Isostatic Press, 0.5cm-thick and with a diameter of 2''.
Al:ZnO (AZO) target composition was 98%ZnO-2%Al2O3 in weight.
Before each deposition, whether i-ZnO or AZO, the chamber was previously pumped down to at least 5∙10-6 mbar by means of a turbopump and then Ar was introduced as process gas. The targets underwent a cleaning process before the growth, avoiding deposition onto the sample by means of a shutter. Once
the deposition. Series to optimize i-ZnO and AZO layers were conducted, in function of distance, sputtering power, Ar pressure and temperature. RT depositions were preferred to avoid element inter-diffusion at the interfaces which were detrimental for the device behaviour. The best growth conditions are shown in Table 5.1:
Table 5.1- Deposition parameters for RF-Magnetron sputtering of i-ZnO and AZO.
Material Distance (cm)
Power (W) / Power density
Deposition Rate (nm/min)
i-ZnO 8 100 / ~5 5∙10-3 RT 15.4
AZO 8 120 / ~6 5∙10-3 RT 32.0
With these settings, the materials were adjusted for the solar cells, both in terms of electrical properties and optical ones. The intrinsic ZnO layer was very resistive, Rsheet>2∙106 Ω/sq. The AZO resistivity was strongly decreased heating the substrate up to 250 °C, but the solar cells suffered of great FF and Voc
drops when heated, so TCO sputtering depositions were performed at room temperature. The best results for AZO deposition at RT by sputtering (Rsheet=10-22 Ω/sq for a thickness of 890 nm, transmittance) are shown in section 5.4.1, along with a comparison with AZO grown by PED.
Unfortunately, in the middle of the PhD project, following to a failure of the cooling system, the cathode overheated and the magnetic field was modified. The new deposition condition resulted in a bad film properties at the centre of the deposition: more resistive Al-ZnO film and highly-stressed i-ZnO, which often ended up in cracks and film crumbling. Thus, from then, the sputtering growths of both materials were carried out in off-axis configuration. Off-axis deposition with the sample centre shifted 2.5 cm from the deposition centre allowed good conductive AZO and resistive i-ZnO without structural problems. Of course, because of the off-axis position, the film thickness was not homogeneous on the surface: the deposition angle from the axis changed from 8.5° on one side of the sample to 25.5° on the other side. As a result, the AZO thickness over the sample varied from 850 nm to 700 nm and its sheet resistance from 45 Ω/sq to 25 Ω/sq (resistivity from 3.8∙10-3 Ωcm to 1.7∙10-3 Ωcm). The thickness variation of i-ZnO was from 100nm to 85nm, and no appreciable variation was observed in its resistivity.
The average optical transmittance of the i-ZnO/AZO bilayer was 85±3%, significantly affected by reflectance due to the thickness of the total window layer (950nm-800nm). In this configuration, small variation in the solar cell behaviour were due to the bad uniformity of TCO thickness and sheet-resistance.
The samples with alternative buffer layer had TCO deposited by DC-sputtering, following another process as described in chapter 7.
5.3.6. Front contacts
Aluminium contacts were thermally evaporated onto the Al:ZnO in a specific chamber. Their thickness is 2 μm. Aluminium (5N) rods for a weight of 0.3 g were loaded in a Ta boat supplied with a DC power of about 400 W. Under these conditions, at a pressure <5∙10-6 mbar, the rods are melted and Al starts to evaporate towards the sample, located at 10 cm from the boat crucible. The sample is placed under a metal shadow mask with different geometries; the most used one for this thesis were made by a circular dot, with a diameter of 1 mm, and one 3mm-long thin finger. The solar cells were then mechanically scribed in rectangular 0.5 cm2, 0.1 cm2 or 0.2 cm2 area with the Al contact in the middle.
The samples with alternative buffer layer and co-evaporated CIGS (section 7.4) had contacts made by Ni/Al/Ni structure in fork geometry. This structure is aimed to reduce the contact resistance between the materials and to prevent Al oxidation, thus giving good and stable contacts over a long time.
Note that no antireflection coating was applied for any solar cells of this thesis.